- Research article
- Open Access
Effect of carboxymethyl cellulose concentration on physical properties of biodegradable cassava starch-based films
© Rachtanapun et al 2011
- Received: 16 September 2010
- Accepted: 10 February 2011
- Published: 10 February 2011
Cassava starch, the economically important agricultural commodity in Thailand, can readily be cast into films. However, the cassava starch film is brittle and weak, leading to inadequate mechanical properties. The properties of starch film can be improved by adding plasticizers and blending with the other biopolymers.
Cassava starch (5%w/v) based films plasticized with glycerol (30 g/100 g starch) were characterized with respect to the effect of carboxymethyl cellulose (CMC) concentrations (0, 10, 20, 30 and 40%w/w total solid) and relative humidity (34 and 54%RH) on the mechanical properties of the films. Additionally, intermolecular interactions were determined by Fourier transform infrared spectroscopy (FT-IR), melting temperature by differential scanning calorimetry (DSC), and morphology by scanning electron microscopy (SEM). Water solubility of the films was also determined. Increasing concentration of CMC increased tensile strength, reduced elongation at break, and decreased water solubility of the blended films. FT-IR spectra indicated intermolecular interactions between cassava starch and CMC in blended films by shifting of carboxyl (C = O) and OH groups. DSC thermograms and SEM micrographs confirmed homogeneity of cassava starch-CMC films.
The addition of CMC to the cassava starch films increased tensile strength and reduced elongation at break of the blended films. This was ascribed to the good interaction between cassava starch and CMC. Cassava starch-CMC composite films have the potential to replace conventional packaging, and the films developed in this work are suggested to be suitable for low moisture food and pharmaceutical products.
- Differential Scanning Calorimetry Thermogram
- Moisture Sorption
- Cassava Starch
The development of biopolymer-based edible films could replace the use of some petrochemicals in the food packaging industry and reduce the negative environmental impact associated with packages from non-renewable and non-recyclable resources. Edible films are generally produced from renewable natural and abundant biodegradable polymeric materials such as polysaccharides, proteins, lipids, or the combination of these components. Some edible films and coatings have been widely used for fresh fruits, vegetables, confectioneries, frozen foods, and meat products . However, many edible films have limitations in mechanical or barrier properties or are prohibitively expensive. Starch films often have good barrier properties to oxygen, carbon dioxide, and lipids and can protect products from lipid oxidation . Films from polysaccharides are also stronger and more extensible than proteinaceous films .
Cassava (Manihot esculenta crantz) or tapioca is one of the economically important crops in Thailand and is the cheapest raw material for starch production. Structurally, cassava starch consists of 17% amylose content, and this is responsible for its strong film-forming characteristics . Cassava starch can readily be cast into films. However, the cassava starch film is brittle and weak, leading to inadequate mechanical properties. Overcoming the brittleness of the film can be accomplished by adding plasticizers . Common plasticizers used in the production of starch films are water, glycerol, sorbitol, and other low-molecular weight polyhydroxy compounds . Glycerol and sorbitol are widely used as plasticizers because of their stability and edibility. The addition of plasticizers makes the brittle films more flexible, but also less strong  and results in higher moisture permeability . This problem must be addressed to improve the functional properties of cassava starch films. Blending  or laminating  with other polysaccharide materials could improve cassava starch film mechanical functionality. Carboxymethyl cellulose (CMC), xanthan, guar, and arabic gum, which are water-soluble heteropolysaccharides with high molecular weights, are often used together with starches to provide desirable texture, control moisture and water mobility, and improve overall product quality and/or stability . CMC is an anionic linear polysaccharide derived from cellulose. It is an important industrial polymer with a wide range of applications in flocculation, drug reduction, detergents, textiles, papers, foods, and drugs . CMC is used primarily because it has high viscosity, is non-toxic, and is non-allergenic. The numerous hydroxyl and carboxylic groups in CMC enable water binding and moisture sorption properties. CMC hydrogel has a high water content, good biodegradability, and a wide range of applications due to its low cost . Because of its polymeric structure and high molecular weight, it can be used as a filler in biocomposite films . CMC is able to improve the mechanical and barrier properties of pea starch-based films .
Some edible films based on mixtures of multiple polysaccharides such as starch-methylcellulose , pullulan-starch , chitosan-starch and chitosan-pullulan , CMC-rice starch , and CMC-pea starch  have been investigated. These publications demonstrated that homogeneous structures containing a single-phase of polymeric complexes have been obtained. Depending on the interactions between components, these formulas can improve the mechanical and moisture barrier properties of the edible films in some cases. In a previous study , water vapor permeability and moisture sorption isotherms of cassava starch based films blended with CMC were studied. The addition of CMC to cassava starch films had no effect on the WVPs of all films tested (WVP ranged from 0.05 to 0.10 and 0.2 to 0.3 g mm/day m2 mmHg at 33% and 54% RH, respectively), but moisture sorption of cassava starch based films increased with increasing CMC contents. It was suggested that the cassava starch based films with and without CMC had potential for use as biodegradable and edible packaging due to the moderate WVP. However, the mechanical properties of biodegradable films are also important for their applications. There is no data available about the physical properties of cassava starch films blended with CMC, thus the objective of this study was to determine the effect of CMC concentration on mechanical and physical properties of cassava starch based films.
The influence of CMC concentrations on properties of cassava starch based films was analyzed in terms of FT-IR spectra, mechanical properties of the films, water solubility, DSC thermograms, and film morphology as reported below. All the cassava starch films with and without CMC appeared smooth, clear, and transparent. Film thickness ranged from 120-160 μm.
The FT-IR spectrum of a CMC film is shown in Figure 1f. The broad absorption band at 3260 cm-1 is due to the stretching frequency of the -COO group  which overlaps with the -OH stretching region at 3480-3440 cm-1. The band at 2876 cm-1 is due to the C-H stretching vibration. The bands around 1412 and 1319 cm-1 are assigned to -CH2 scissoring and -OH bending vibration, respectively. The band at 1060 cm-1 is due to CH-O-CH2 stretching . Spectra of CMC films showed peaks around 1592 cm-1, attributable to antisymmetric vibration of COO- groups [21, 22].
Adding a range of CMC concentrations to cassava starch films resulted in similar characteristics in the FT-IR spectra (Figures 1b, c, d and 1e). Blending CMC with cassava starch caused minimal shifting but increased absorption in the COO- band around 1592 cm-1 in cassava starch films containing 10, 20, 30 and 40% CMC, respectively. This indicated that the antisymmetric and symmetric vibrations of C = O and C-O bonds were enhanced, probably due to the disruption of intermolecular H-bonds between carboxylic groups caused by added starch . The symmetric COO- stretching was found at ~1411 cm-1 in all film samples. The water absorption band of cassava starch at 1648 cm-1 disappeared upon addition of CMC. The broad band located around 3270 cm-1 appeared in all films and was caused by O-H stretching and intermolecular/intramolecular hydrogen bonds [23, 24]. The O-H band of CMC and cassava starch occurred at 3267 and 3261, respectively. By blending cassava starch with CMC, the O-H band of films shifted to 3265-3272 cm-1. The band of C-OH bending of cassava starch film that appeared at 1337 cm-1 was shifted to 1322-1333 cm-1 with CMC addition. Xu et al.  reported that the ester bonds were mostly formed between the hydroxyl groups in amylopectin branches of starch and carboxylic acid groups of CMC, forming a stable cross-linked structure. This is likely what occurred in the composite cassava starch CMC films studied here. These results were correlated with FT-IR spectra of rice flour-CMC blended film , chitosan-cassava starch-gelatin films , and corn starch-CMC-nanoclay biocomposite films .
The tensile strength and elongation at break of cassava starch based films were inversely related. At 34% RH, cassava starch based films containing CMC had significantly higher tensile strength but lower elongation at break than control films (cassava starch film without CMC). As the concentration of CMC increased, the tensile strengths of films significantly increased but the elongations at break significantly decreased. These results were consistent with corn starch films  and pea starch films  which had improved tensile strength as the concentration of added CMC increased. The increasing tensile strength of the cassava starch films with increasing concentrations of CMC is likely attributable to the formation of intermolecular interaction between the hydroxyl group of starch and carboxyl group of CMC . During the processing and drying of the composite films, the original hydrogen bonds formed between starch molecules could be replaced by new hydrogen bonds formed between the hydroxyl groups in starch molecules and the hydroxyl and carboxyl groups in CMC . Intermolecular interaction between starch and CMC resulted in more compact molecule structure of starch-CMC mixture, and tensile strength was therefore increased . This finding corroborates the FT-IR results reported above. These results are similar to reports of the tensile strength of chitosan-starch films , rice starch-CMC film , and corn starch-CMC-nanoclay films . At 54% RH, the tensile strength of all films decreased but % elongation increased when compared with the films at 34% RH. Gennadios et al.  reported that films with higher elongation values usually require a lower load to cause film breakage. These results could be related to structural modification of the starch network by water which causes a greater flexibility in polymer structure. At 54% RH, increasing CMC concentration in the cassava starch films improved the tensile strength but reduced the elongation at break. This result agreed with effect of humidity on tensile strength and % elongation of blended chitosan-methylcellulose films .
Solubility in water is an important property of starch-based films. Potential applications may require water insolubility to enhance product integrity, moisture barrier properties, and shelf-life. However, in other cases the water solubility of films before product consumption might be useful, such as for the encapsulation of food ingredients or additives .
Composition of CMC/cassava starch in 100 ml film solution
Composition (g/100 ml water)
Melting temperature and heat of fusion of cassava starch film without and with CMC
Tm starch-CMC film (°C)
Heat of fusion (ΔHf) of starch-CMC film (J/g)
Cassava starch: CMC (100:0)
Cassava starch: CMC (90:10)
Cassava starch: CMC (80:20)
Cassava starch: CMC (70:30)
Cassava starch: CMC (60:40)
Cassava starch: CMC (0:100)
The melting temperature (Tm) of cassava starch films blended with CMC were lower than the Tm of cassava starch films but higher than the Tm of CMC films (except for the film with 40% CMC). The Tm of film blends shifted due to the interaction of the two biopolymers . The area under the endothermic peak expressed the total heat of fusion of the films [32, 33], which increased with increasing CMC concentrations in cassava starch films. The increased heat of fusion should be the effect of higher crystallization because of the high degree of crystallinity of CMC . The total heat of fusion of blended films was lower than for CMC alone, likely because the interaction between cassava starch and CMC molecules interrupted the rearrangement of polymer chains . Gimeno et al.  found that a higher interaction of hydrocolloids and starch retained more water molecules, causing a higher mobility during heating, increasing the kinetic energy, and decreasing the enthalpy value (ΔH). These results were similar to DSC thermograms of HDPE/PP blends  and chitosan-MC films with vanillin .
The effects of CMC concentrations and relative humidity on physical properties of cassava starch based films were studied. The addition of CMC to the cassava starch films increased tensile strength and reduced elongation at break of the blended films. This was ascribed to the good interaction between cassava starch and CMC. FT-IR spectra indicated intermolecular interactions between cassava starch-CMC film blends by shifting of carboxyl (C = O) and OH groups. The thermogram of film blends also confirmed chemical interaction of cassava starch-CMC as ΔH decreases. The homogeneity of cassava starch-CMC films was represented as a single melting peak, and SEM micrographs visibly confirmed the homogeneous structure of cassava starch-CMC films. All films stored at 54% RH gave higher elongation but lower tensile strength than films at 34% RH. Increasing CMC concentrations in the cassava starch film decreased water solubility of the blended films. Films containing 30% CMC had better physical properties (high tensile strength, moderate elongation and low water solubility) than the other films. Thus, it seems that the CMC-starch biocomposite films show better physical properties than cassava starch films alone, and cassava starch-CMC composite films have the potential to be used as edible and biodegradable films for low and intermediate moisture products.
Cassava starch (Bangkok Inter Food Co., LTD., Thailand) and glycerol (EM Science, Germany) were employed to produce the films. CMC was donated from Akzo Nobel (Netherlands).
Cassava starch-CMC film preparation
Solutions used to prepare films (5% w solid/v) were prepared by dispersing cassava starch and CMC at different concentrations in distilled water (Table 1). Glycerol (30% w/w solid) was added as the plasticizer. The film solutions were heated to 80°C with constant stirring to obtain starch gelatinization. Then the film-forming solutions (200 ml) were cast on flat 30 × 30 cm Teflon plates. The films were dried at room temperature (25°C) for 24 hours .
Films were cut into 25 × 100 mm strips and then equilibrated in desiccators over saturated salt solutions having the desired relative humidity 34% (MgCl2) and 54% RH (Mg(NO3)2) condition at 25°C for 48 hours before testing. The tensile strength and elongation at break of the films were measured using a universal testing machine (Hounsfield, England) according to the ASTM D 882-91 method . The initial gauge length was 50 mm and crosshead speed was 50 mm/min. Ten specimens were tested for each sample.
Water solubility of cassava starch-CMC films
Fourier transform infrared spectroscopy (FT-IR)
Transmission infrared spectra of the films were recorded at room temperature using a Nicolet 6700 FT-IR spectrometer (Thermo Electron Corporation, USA) in the range of 4000-400 cm-1 with 64 scans, 4 cm-1 resolution, using a DTGS KBr detector and KBr beam splitter. The films were mounted directly in the sample holder.
Differential scanning calorimetry (DSC)
Differential scanning calorimetry was carried out using a Mettler Toledo Schwerzenbach instrument (USA). Samples were previously conditioned at 54% RH and 25°C. Three replicates of film samples (~10 milligrams) contained in aluminum pans were heated in the temperature range -20 to 220°C at a heating rate of 5°C/min in a nitrogen atmosphere (50 ml/min).
Film samples were conditioned at 25°C in 54%RH desiccators for 7 days prior to analysis. The surface and cross-section microstructure of films were observed by Field-Emission Scanning Electron Microscope (FESEM, JOEL JSM-6700F, Japan).
ANOVA analysis was performed on all results using a statistical program SPSS v. 10.0 at a confidence interval of 95% to determine the significant difference between group samples.
The authors gratefully acknowledge the National Research University Project under Thailand's Office of the Higher Education Commission (CHE), Thailand for financial support. The authors also thank Akzo Nobel (Netherlands) for CMC donation.
- Ou S, Wang Y, Tang S, Huang C, Jackson MG: Role of ferulic acid in preparing edible films from soy protein isolate. J Food Eng. 2005, 70: 205-210. 10.1016/j.jfoodeng.2004.09.025.View ArticleGoogle Scholar
- Banker GS: Film coating theory and practice. J Pharm Sci. 1966, 55: 81-89. 10.1002/jps.2600550118.View ArticleGoogle Scholar
- Krochta JM, De Mulder CLC: Biodegradable polymers from agricultural products. Agricultural Materials as Renewable Resources. Edited by: Fuller G, McKeon TA, Bills DD. 1995, Washington, DC.: American Chemical Society, 120-140.Google Scholar
- Bangyekan C, Aht-Ong D, Srikulkit K: Preparation and properties evaluation of chitosan-coated cassava starch films. Carbohydr Polym. 2006, 63: 61-71. 10.1016/j.carbpol.2005.07.032.View ArticleGoogle Scholar
- Suppakul P, Chalernsook B, Ratisuthawat B, Prapasitthi S, Munchukangwan K: Plasticizer and Relative Humidity Effects on Mechanical Properties of Cassava Flour Films. The 15th IAPRI World Conference on Packaging; 3 - 5 October 2006 Tokyo, Japan. 2006Google Scholar
- Rindlav-Westling A, Stading M, Hermansson AM, Gatenholm P: Structure, mechanical and barrier properties of amylose and amylopectin films. Carbohyd Polym. 1998, 36: 217-224. 10.1016/S0144-8617(98)00025-3.View ArticleGoogle Scholar
- Kester JJ, Fennema O: Edible films and coatings: a review. Food Technol. 1986, 40: 47-59.Google Scholar
- Chandra R, Rustgi R: Biodegradable polymers. Prog Polym Sci. 1998, 23: 1273-1335. 10.1016/S0079-6700(97)00039-7.View ArticleGoogle Scholar
- Coffin DR, Fishman ML: Viscoelastic properties of pectin/starch blends. J Agr Food Chem. 1993, 41: 1192-1197. 10.1021/jf00032a005.View ArticleGoogle Scholar
- Li Y, Shoemaker CF, Ma J, Shen X, Zhong F: Paste viscosity of rice starches of different amylose content and carboxymethylcellulose formed by dry heating and the physical properties of their films. Food Chem. 2008, 109: 616-623. 10.1016/j.foodchem.2008.01.023.View ArticleGoogle Scholar
- Biswal DR, Singh RP: Characterisation of carboxymethyl cellulose and polyacrylamide graft copolymer. Carbohyd Polym. 2004, 57: 379-387. 10.1016/j.carbpol.2004.04.020.View ArticleGoogle Scholar
- Nie H, Liu M, Zhan F, Guo M: Factors on the preparation of carboxymethycellulose hydrogel and its degradation behaviour in soil. Carbohyd Polym. 2004, 58: 185-189. 10.1016/j.carbpol.2004.06.035.View ArticleGoogle Scholar
- Almasi H, Ghanbarzadeh B, Entezami AA: Physicochemical properties of starch-CMC-nanoclay biodegradable films. Biol Macromol. 2010, 46: 1-5. 10.1016/j.ijbiomac.2009.10.001.View ArticleGoogle Scholar
- Ma X, Chang PR, Yu J: Properties of biodegradable thermoplastic pea starch/carboxymethyl cellulose and pea starch/microcrystalline cellulose composites. Carbohyd Polym. 2008, 72: 369-375. 10.1016/j.carbpol.2007.09.002.View ArticleGoogle Scholar
- Arvanitoyannis I, Biliaderis CG: Physical properties of polyol-plasticized edible blends made of methyl cellulose and soluble starch. Carbohyd Polym. 1999, 38: 47-58. 10.1016/S0144-8617(98)00087-3.View ArticleGoogle Scholar
- Biliaderis CG, Lazaridou A, Arvanitoyannis I: Glass transition and physical properties of polyol-plasticised pullulan-starch blends at low moisture. Carbohyd Polym. 1999, 40: 29-47. 10.1016/S0144-8617(99)00026-0.View ArticleGoogle Scholar
- Lazaridou A, Biliaderis CG: Thermophysical properties of chitosan, chitosan-starch and chitosan-pullulan films near the glass transition. Carbohyd Polym. 2002, 48: 179-190. 10.1016/S0144-8617(01)00261-2.View ArticleGoogle Scholar
- Tongdeesoontorn W, Mauer LJ, Wongruong S, Rachtanapun P: Water vapour permeability and sorption isotherm of cassava starch based films blended with gelatin and carboxymethyl cellulose. Asian J Food Agro-Ind. 2009, 2: 501-514.Google Scholar
- Vicentini NM, Dupuy N, Leitzelman M, Cereda MP, Sobral PJA: Prediction of cassava starch eible film properties by chemometric analysis of infrared spectra. Spectrosc Lett. 2005, 38: 749-767. 10.1080/00387010500316080.View ArticleGoogle Scholar
- Su JF, Huang Z, Yuan XY, Wang XY, Li M: Structure and properties of carboxymethyl cellulose/soy protein isolate blend edible films crosslinked by Maillard reactions. Carbohyd Polym. 2010, 79: 145-153. 10.1016/j.carbpol.2009.07.035.View ArticleGoogle Scholar
- Xiao C, Weng L, Zhang L: Improvement of physical properties of crosslinked alginate and carboxymethyl konjac glucomannan blend films. J App Polym Sci. 2002, 84: 2554-2560. 10.1002/app.10582.View ArticleGoogle Scholar
- Yang F, Li G, He YG, Ren FX, Wang Gx: Synthesis, characterization, and applied properties of carboxymethyl cellulose and polyacrylamide graft copolymer. Carbohyd Polym. 2009, 78: 95-99. 10.1016/j.carbpol.2009.04.004.View ArticleGoogle Scholar
- Tong Q, Xiao Q, Lim LT: Preparation and properties of pullulan-alginate-carboxymethylcellulose blend films. Food Res Int. 2008, 41: 1007-1014. 10.1016/j.foodres.2008.08.005.View ArticleGoogle Scholar
- Jiang L, Li Y, Wang X, Zhang L, Wen J, Gong M: Preparation and properties of nano-hydroxyapatite/chitosan/carboxymethyl cellulose composite scaffold. Carbohyd Polym. 2008, 74: 680-684. 10.1016/j.carbpol.2008.04.035.View ArticleGoogle Scholar
- Xu YX, Kim KM, Hanna MA, Nag D: Chitosan-starch composite film: preparation and characterization. Ind Crop Prod. 2005, 21: 185-192. 10.1016/j.indcrop.2004.03.002.View ArticleGoogle Scholar
- Zhong QP, Xia WS: Physicochemical properties of edible and preservative films from chitosan/cassava starch/gelatin blend plasticized with glycerol. Food Technol Biotechnol. 2008, 46: 262-269.Google Scholar
- Ghanbarzadeh B, Almasi H, Entezami AA: Physical properties of edible modified starch/carboxymethyl cellulose films. Innov Food Sci Emerg. 2010, 11: 697-702. 10.1016/j.ifset.2010.06.001.View ArticleGoogle Scholar
- Gennadios A, Weller CL, Testin RF: Property modification of edible wheat gluten films. Trans ASAE. 1993, 36: 465-470.View ArticleGoogle Scholar
- Rachtanapun P, Wongchaiya P: Effect of relative humidity on mechanical properties on blended chitosan-methylcellulose film. Mae Fah Luang Symposium; 26-28 Nov Chiang Rai, Thailand. 2008, 50-Google Scholar
- Bertuzzi MA, Castro Vidaurre EF, Armada M, Gottifredi JC: Water vapor permeability of edible starch based films. J Food Eng. 2007, 80: 972-978. 10.1016/j.jfoodeng.2006.07.016.View ArticleGoogle Scholar
- Veiga-Santos P, Oliveira LM, Cereda MP, Scamparini ARP: Sucrose and inverted sugar as plasticizer. Effect on cassava starch-gelatin film mechanical properties, hydrophilicity and water activity. Food Chem. 2007, 103: 255-262. 10.1016/j.foodchem.2006.07.048.View ArticleGoogle Scholar
- Rachtanapun P, Selke SEM, Matuana LM: Effect of the high-density polyethylene melt index on the microcellular foaming of high-density polyethylene/polypropylene blends. J Appl Polym Sci. 2004, 93: 364-371. 10.1002/app.20428.View ArticleGoogle Scholar
- Sangsuwan J, Rattanapanone N, Rachtanapun P: Effect of vanillin and plasticizer on properties of chitosan-methyl cellulose based film. J Appl Polym Sci. 2008, 109: 3540-3545. 10.1002/app.28461.View ArticleGoogle Scholar
- Gimeno E, Moraru CI, Kokini JL: Effect of xanthan gum and CMC on the structure and texture of corn flour pellets expanded by microwave heating. Cereal Chem. 2004, 81: 100-107. 10.1094/CCHEM.2004.81.1.100.View ArticleGoogle Scholar
- ASTM International: Standard test methods for tensile properties of thin plastic sheeting. Annual book of ASTM. 1991, Philadelphia: American Society for Testing and Materials, D882-91Google Scholar
- Phan TD, Debeaufort F, Luu D, Voilley A: Functional properties of edible agar-based and starch-based films for food quality preservation. J Agr Food Chem. 2005, 53: 973-981. 10.1021/jf040309s.View ArticleGoogle Scholar
- Veiga-Santos P, Suzuki CK, Cereda MP, Scamparini ARP: Microstructure and color of starch-gum films: Effect of gum deacetylation and additives. Part 2. Food Hydrocolloid. 2005, 19: 1064-1073. 10.1016/j.foodhyd.2005.02.007.View ArticleGoogle Scholar